The slope * β*, the Hurst parameter

*, and the fractal dimension*H

*, for two corrosion signals (Planinšič & Petek, 2008).*D

Open access peer-reviewed chapter

By Peter Planinšič and Aljana Petek

Submitted: June 21st 2010Published: September 12th 2011

DOI: 10.5772/intechopen.84034

Downloaded: 1839

Electrochemical noise (EN) is the term used to describe the spontaneous fluctuations of current or potential, which are generated during the corrosion processes. It has been investigated extensively since the 1968, and data has shown the use of EN measurements offers valuable sources of information about complex electrochemical reactions such as those in corrosion systems (Gabrielli et al., 1985; Bertocci & Huet, 1995).

Many methods can be used to analyze the data, such as the variance, standard deviation and root mean square in the time domain. Alternatively, the signal has been transformed from the time domain to the frequency domain using fast Fourier transform or the maximum entropy method, giving the power spectrum density (PSD). The technique of wavelet analysis may be used instead, where a set of wavelets of varying amplitude, duration, and location be constructed such that reproduces the signal of interest.

Wavelets based methods are modern mathematical tools for multiscale time frequency analysis and characterization of in general nonstationary EN signals. This work presents the short overview to usability and possibilities of wavelet transformation in comparison with classic analysis.

Advertisement## 2. Corrosion processes and electrochemical noise

Fe → Fe 2 + + 2e − E12 H + + 2e − → H 2 E2O 2 + 4 H + + 4e − → 2 H 2 O E3Fe + 2 H + → Fe 2 + + H 2 E42 Fe + O 2 + 4 H + + 4e − → 2 Fe 2 + + 2 H 2 O E5j = j 0 { e ( 1 − α ) f η − e − α f η } E6f = n F R T E7

Corrosion can be defined as the deterioration of materials due to its interaction with its environment and is appearing in various forms: as localized corrosion and as general (uniform) corrosion. Localized corrosion results in the accelerated loss of material at discrete sites in a passive materials surface, leading to the perforation or other failure. Since the majority of the surface is unaffected the difficulty with localized corrosion is its detection and prediction. Uniform corrosion results from the sites that are distributed randomly over the surface regarding both the space and time. Uniform corrosion damage is manifested in dissolving and the progressive thinning of a metal. To prevent corrosion or to predict the outcome of a corrosion situation the knowledge of mechanism of various form of corrosion is fundamental. Thermodynamic principles can be applied to determine which processes can occur and how strong the tendency is for changes to take place. Kinetic laws then describe the rates of the reactions.

Corrosion of metals in aqueous environments is electrochemical in nature. It occurs when two or more electrochemical reactions take place on a metal surface, producing dissolved species of metal or solid corrosion products and thus lowering the energy of the system. The corrosion process has been written as two separate reactions occurring at two distinct sites on the same surface: the anode (metal dissolution site) and the cathode (site of the accompanying reduction reaction). At corrosion of iron in an acid solution containing dissolved oxygen, iron is oxidized to ferrous ion which passes into solution in the anode region

and H^{+} ion is reduced to hydrogen or O_{2} is reduced to water in the cathode region

The overall corrosion reaction is the sum of the anodic and cathodic partial reactions:

sum of the reactions (1) and (2)

and sum of the reactions (1) and (3)

Electrochemical corrosion processes can be investigated by observation of charge flows between the electrolyte and the corroding metal. The measure of the rate at which reducible or oxidizable species can gain or lose electrons is the current density,

where

where * F*is Faraday constant,

In measurements procedure a potentiostat is often used and the electrochemical cell with tree electrodes: working electrode (WE) represents the interface of interest, the reference electrode (RE) acts as standard for potential measurements and the counter electrode acts as electron sink or source for reactions that occur on the surface of WE. The potential of the WE is controlled with respect to the RE at a constant value, and the current density

In our investigations the current noise was monitored by a low-noise battery-operated potentiostat Jaissle IMP88 PC-R at a sampling rate of 10 points per second. The cell assembly was put in a Faraday cage. An example of measured time series for two processes (pitting as signal _{0} and general corrosion as signal _{2}) is presented in Fig. 1. As is seen, the signal has a relatively smooth appearance for general corrosion and occasional sharp increases and decreases in the amplitude of current noise data occur for localized corrosion.

EN-signals are generated from corrosion processes which are stochastic in their nature. A short theoretical overview of stochastic processes follows (Schroeder, 1991; Flandrin, 1992; Gao et al., 2007).

For understanding the stochastic processes it is essential to understand the concept of probability which is associated with random events. Often random events are presented by numbers, called a random variable. Let us denote a random variable by * X*, whose value depends on the outcome of random experiment

The mean or average of * X*can be obtained by relation:

The p^{th} order moment of * X*around zero is defined as:

The second moment represents the power of a random variable * X*.

The p^{th} order central moment of * X*around mean value is defined as:

Variance of * X*is denoted as

For a a given sample space * S*, a set of events

The activity of complex systems can usually be characterized by appearance of * β*is the power spectral exponent. A convenient framework for studying

where * H*is the Hurst parameter which is the measure of self-similarity. It can be derived, that a mean of such process is:

the variance

and autocorrelation

By proving that * f*property:

where * ω*is radial frequency,

An example of self-affine stochastic process is fractional Brownian motion process (fBm). It is nonstationary zero mean Gaussian process denoted as* H*(Hurst parameter). The nonstrationary characteristic of fBm is evident from its covariance function structure:

where * E*is the expectation operator. From this covariance function follows that the variance is of the type:

Although fBm process is nonstationary, it has stationary increments, which means that the probability properties of the difference process * t*-

The other example of

It was reported, that * β*is related to the Hurst parameter

This is the reason for studying * H*is related to fractal dimension

* D*is noninteger parameter in the range

Let * S*be a bounded set in

In the past, the most common EN-analysis methods were statistical and Fourier methods. These methods assume the stationary or quasi stationary nature of processes and signals under consideration.

An early overview of different EN-data analysis methods was made in the work by R. A. Cottis (Cottis, 2001). Follows a little extended theoretical overview of classical methods (Orfanidis, 1996).

By analyzing random processes the statistical parameters as mean value and moments are defined by expectation operators, i.e. by statistical averaging of many realizations of stochastic process. In practice this is many times impossible and there is available only one block or array of * N*time signal samples. The statistical averaging is then replaced by the estimation obtained using sample or time average.

The p^{th} moment of sample * x*(

The first moment is mean value_{rsm}, which measures the amplitude of the signal. The square of _{rsm} represents the signal power.

The p^{th} central moment of sample is defined as:

The second order central moment is the well known signal variance. The square root of variance is standard deviation, which is usually used for describing the amplitude of noise signals.

Classical spectral analysis bases on Fourier transform. The Fourier Transform of the deterministic continuous time signal * x*(

The Discrete Time Fourier Transform (DTFT) of the deterministic sampled signal with * N*samples is defined as:

where * x*(

where * n*is time index and

where _{s} is radial sampling frequency. The main shortcoming of classical Fourier transform is the averaging the features across the whole time domain.

EN signals are of stochastic nature; therefore sampled EN signals are random sequences. To obtain smooth spectra an ensemble averaging should be introduced and the spectrum calculated over autocorrelation function. The autocorrelation function of a zero mean random signal is defined as:

where * E*is the averaging or expectation operator. For stationary signals,

where * ω*is the frequency in radians per sec. This power spectrum shows how the power is spread over frequencies and is also called PSD (Power Spectral Density).

EN measurements cannot often be repeated to obtain smoothed spectra by ensemble averaging. One can compute an estimate of expected or true value by so-called sample autocorrelation using time average:

for * k*=0,1,…

The DTFT of

Using the above equations we can express the periodogram also as:

where * N*signal samples. It can be efficient computed using FFT. For wide sense stationary random signals the mean of periodogram converges to the true power spectrum

There are some problems with such classical Fourier spectral analysis method. To achieve high statistical reliability, very long signal sequences should be used. But long signal sequences can no longer be stationary. However, the main shortcoming is the averaging the futures over the whole time domain.

This have lead researchers to find and develop of an advanced signal analysis methods. Recently wavelet based methods for signal analysis found to be useful for nonstacionary signals. Therefore in this overview chapter we will consider wavelet-based methods for EN-signals analysis.

In individual systems, the correlations between noise measurements and corrosion processes have been reported by many authors but only some can be mentioned here. The EN data for a passive system (SS 316L/Ringer′s solution) and several active systems (mild steel/NaCl, brass/NaCl, Al 6061/NaCl and Al 2024/NaCl) have been analyzed in the frequency domain using power spectral density (PSD) and spectral plots, obtained from the ratio of PSD plots of the potential and current fluctuations. Comparisons of spectral noise spectra with traditional impedance spectra have been made and good agreement has been observed for all systems after trend removal (Lee & Mansfeld, 1998; Mansfeld et al., 2001). Current fluctuation during general corrosion was analyzed upon a simple model, derived on the assumption that elementary fluctuation sources are related to the fluxes of electrons that are transferred from the metal to electron-acceptor ions in solution. The number of successful electron transfers obeyed a Gaussian distribution, from which the corrosion current density and transfer coefficients were determined (Petek et al., 1997; Petek & Doleček, 2001). The time-series noise patterns of the steel in bicarbonate solution (the simulated geological environment) were transformed into frequency domain by fast Fourier transformations, and then their power spectral densities at a frequency were determined to be compared with the corrosion rate (Haruna et al., 2003). Two new indices (S_{E} and S_{G}) were derived to evaluate pitting corrosion by dimensional analysis of three parameters of PSD, the slope of high frequency linear region, the critical frequency and the low-frequency plateau level. As shown, the value of S_{E} can be related to the fluctuation velocity, which can represent the pitting corrosion rate and S_{G} should contain some information about slow corrosion processes (Shi et al., 2008). PSD had been employed to analyze EN data associated with corrosion behavior of A291D magnesium alloy in alkaline chloride solution. Three corrosion stages, the anodic dissolution process companying with the growth, absorption and desorption of hydrogen bubbles, the development of pitting corrosion, and the inhibition process by protective MgH_{2} film could be distinguished. However, the results obtained only from PSD was insufficient for better understanding the corrosion mechanism of alloy during the immersion and the wavelet transform was carried out (Zhang et al., 2007).

EN signal (Fig. 1) is represented as a time series, where one can easily distinguish the fluctuations but not the intensity and frequencies of fluctuations. In the paper (Planinšič & Petek, 2003) we analyzed EN corrosion signals also with some classical methods, which use correlation functions and histograms. Figure 2 shows estimated autocorrelation functions of two corrosion signals _{0} and _{2}, respectively.

Noise data were transformed into frequency domain using FFT algorithm and presented as PSD in Figure 3. PSD of current noise data for pitting process exhibited two parts: a low-frequency plateau and high-frequency part, and the roll-off frequency, which is the frequency to separate the two parts of PSD. PSD plot of general corrosion can be characterized by “white noise” which is independent of frequency.

Amplitude distribution was studied using normalized histograms. As demonstrated by Figure 4, a current noise amplitude distribution of general corrosion is Gaussian.

The assumption of stationary behavior of corrosion processes and random signals is not always correct. Corrosion signals are a non stationary in general.

When we are interested on how signal frequency components vary with time, we should use joint time-frequency analysis. For this purpose we can use Window Fourier Transform (WTF), also called Short Time Fourier Transform (STFT) or spectrogram. It is known that the STFT can be considered as the filter bank, consists of Finite Impulse Response Filters (FIR) with equal bandwidth or equal frequency resolution. Therefore it is difficult to meet sharp localization in time and frequency simultaneously. For this reason, this technique is not always appropriate for analyzing natural signals or phenomena, where in the signal exist long duration low frequency components and short high frequency components at the same time. This problem can be elegantly solved using modern multiresolution time frequency analysis methods based on wavelets. It was shown that the Discrete Wavelet Transform can be viewed and realized as multirate filter bank with octave, also called constant * Q*frequency resolution.

A short theoretical overview of wavelet methods follows (Daubechies, 1992; Burrus, 1992; Fladrin,1992, 1993; Radolphe, 1994; Wornell, 1996; Mallat, 1998; Dai et al., 1994; Palawajjhalla et al., 1994).

Wavelets are waves which construct basis of signal decomposition in wavelet transforms, similar as trigonometric functions with different frequencies in Fourier Transform. Wavelets are scaled and shifted versions of the so called mother or primary wavelet function

where parameters * a*and

where

Admissibility implies that a wavelet must be an oscillatory decaying function with zero mean. There are also additional other desirable properties for a function to be a useful wavelet, as smoothness, good time and frequency localization, number of vanishing moments. These properties suggest that wavelets are bandpass filters.

In the contrast with Fourier analysis where basis functions are trigonometric functions, by wavelet-based analysis different kind of mother wavelet function can be used, appropriate for particular application. There are many types of wavelet transforms according to input signals, time and scaling parameters, used wavelet functions, namely continuous, discrete, bi-orthogonal and semi-orthogonal and orthonormal bases version.

However wavelet transform can be broadly classified into Continuous Wavelet Transform (CWT) and Discrete Wavelet Transform (DWT). CWT of a function

Discrete wavelet transform involves discretization of parameters, * a*and

where

are called frames (Daubechies,1992) and form Riesz basis. Discrete wavelets can be further classified into orthogonal, semi-orthogonal or non-orthogonal.

To obtain orthonormal basis, one can chose samples on dyadic grid (base 2):

Orthonormal bases and orthonormal wavelet transform, play an important role in theory and practice of multiresolution analysis. The DWT can be further classified into Wavelet Series Transform (WST), when analyzed signal is continuous (* f*(

where * h*(

where the finite sequence * g*(

The multiresolution analysis form the theoretical basis for fast Discrete Wavelet Transform (fast DWT), using discrete signals * f*(

* T*he sequences at scale

where * j*=1 represents approximated or smoothed version of the original signal. The sequence

For EN-signal originating from corrosion process, wavelet transform decompose it into approximation and detail signal components at different scales and locations. The wavelet transform is therefore convenient tool to analyze the self-similarity of 1/f time series.

The orthonormal wavelet transform based methods were used for estimating slope* H*, and fractal dimension

where _{j} ^{2} is the variance of detail signal* β*can be calculated from the plot

Wavelets have found many applications in different natural scientific disciplines, among them also in chemical engineering (Radolphe et al., 1994; Banjanin et al., 2001). The use of wavelets to study electrochemical noise transients was reported by Aballe (Aballe et al., 1999; 2001). The wavelet analysis of electrochemical noise signals, where the signal was decomposed into wavelet-subbands was used for the characterization of pitting corrosion intensity (Smulko et al., 2002). Wharton et al. demonstrated how the wavelet variance exponent can be used to evaluate corrosion behavior for variety of stainless steels in chloride medium, i.e. be able to discriminate between various corrosion processes covering a wide range of EN signals (Wharton et al., 2003). Wavelet analysis based on the fractional energy contribution of smooth crystals and the lowest frequency detail crystal can provide information on the type and onset of corrosion (general corrosion, metastable pitting, stable pitting) in performed potentiostatic critical pitting temperature test for a superduplex stainless steel (Kim, 2007). In study of the copper anode passivation by electrochemical noise analysis using wavelet transforms it has been found that during active dissolution the electrode surface is dominated by long time scale process and the change of the position of the maximum relative energy from D7 to D8 could be an indication of future passivation (Lafront et al., 2010). It was shown, that electrochemical potential noise analysis of Cu-BTA system using wavelet transformation can be used to achieve the inhibition efficiency (Attarchi et al., 2009).

Some other authors also reported about the fractal nature of corrosion processes and corresponding electrochemical noise signals. The electrochemical potential and current noise originating from the corrosion of carbon steel in distilled water was analyzed using multifractal analysis. The multifractal spectra are found to be qualitatively different for different temporal stages of the corrosion process (Muniandy et al., 2011).

Our applications of wavelets transformation or combination with classical methods for the electrochemical current noise analysis were reported for different corrosion processes in several publications (Planinšič & Petek, 2003; 2004; 2007; 2008). For little more detailed insight the short overview of this research is as follows.

Daubechies wavelets ‘’db2’’ were used to transform the EN signal from Fig. 1. The discrete wavelet transform (DWT) decomposition of signal into on joint time (position) and frequency (scale level) depended amplitudes are presented with color lightness in time-frequency plane in Fig. 6.

Next, the DWT multiresolution decomposition of processes on 5 levels are shown in Fig. 7. The crystals from _{1} to _{5} are the details of the signal, and _{5} is the approximation of the signal. The frequency range which takes into account each series of detail coefficients, can be computed from relation_{s} is the sampling frequency and * j*stands for the corresponding scale.

Events with small time constants are taken into account by the fine scale coefficients, details _{1}, _{2}. The information dealing with larger time constant events is included in details _{4} and _{5}. Therefore, these kinds of plot allow the signal to be viewed over the full time range and considering different scales, which contains information about corrosion events occurring at a determined time – scale.

Variances of details were calculated to detect the intensity of particular signal components on level * j*. Fig. 8 shows variances as a function of the decomposition level and also the logarithmic plot of details variances versus level

For the time series _{2} and _{0} were * ß*= 0.7700 and

After short computation the value for Hurst parameter * H*, and fractal dimension

The obtained slope * ß*is the estimated power spectral exponent

The obtained results indicating the presence of fractional Brownian motion in pitting corrosion with adjacent values in the time series being strongly correlated and fractional Gaussian noise in general corrosion, with adjacent values in the time series being weak correlated. The Hurst parameter in case of pitting is greater than ½, indicating also the persistence, i.e. a dependence of new values on old values. A summary of the wavelet – based fractal analysis is given in Table 1.

_{i} | _{i} | _{i} | process | persistence | |

_{0} – pitting corrosion | 3.0092 | 1.0046 | 0.9954 | non- stationary | strong |

_{2} – general corrosion | 0.7700 | -0.1150 | 2.1150 | stationary | weak |

We proposed also a new way for determination of persistence nature of the electrochemical noise on the basis of correlation coefficients between original signal and details * R*(

(_{0},_{j}) | (_{2},_{j}) | |

_{1} | 0.0188 | 0.4196 |

_{2} | 0.0482 | 0.5303 |

_{3} | 0.1128 | 0.5097 |

_{4} | 0.2048 | 0.3648 |

_{5} | 0.3103 | 0.3138 |

Correlation coefficients between successive details * R*(

_{0} | _{2} | |

(_{1},_{2}) | 0.0006 | 0.0006 |

(_{2},_{3}) | 0.0000 | 0.0004 |

(_{2},_{3}) | 0.0001 | 0.0004 |

(_{4},_{5}) | -0.0012 | -0.0120 |

Additionally, DWT with 3-decomposition levels was made using different kinds of wavelet functions, from Daubechie’s fractal-like wavelet “db2” (Massopust, 1994) to smoother wavelet functions, as Daubechie’s wavelet function “db5” and symmetrical Coiflet wavelet function “coif5”. After decomposition the coding gain (_{g}) was calculated from variances of decomposed sub-bands:

where * J*the number of sub-bands. The coding gain is a measure of spectral flatness. For (uniform) white noise it has the value 1. Also the Shannon’s entropy was calculated and can be viewed as a measure of signal complexity. The numerical experimental results are collected in Table 4.

_{g}, _{2} | _{g}, white noise | entropy, _{2} | entropy, white noise | |

db2 | 1.3486 | 1.0090 | 4.5384 | 4.9304 |

db5 | 1.3411 | 1.0076 | 4.5384 | 4.9304 |

coif5 | 1.3411 | 1.0116 | 4.5384 | 4.9304 |

The chose of different wavelets did not influence on the obtained _{g} and entropy. We found also, that the coding gain and entropy can be used as an additional parameter to distinguish the corrosion processes.

To study the approximation properties of DWT’s using different wavelet basis functions, a synthesis (inverse DWT) to different approximation levels was made. We expected better results with ‘’db2’’ assuming the fractal–like shapes of EN-signals. However, no significant differences were found, a smaller approximation error was obtained even using smoother wavelets, what confirms the approximation theory.

Advertisement## 6. Conclusion

The most attractive prospective benefit of EN measurement is the ability to obtain information about the type of corrosion that is occurring, but there is much less agreement about the optimum analysis method for obtaining such information (Cottis, 2006). Wavelet transform has been developed over a number of years and only recently has been applied to electrochemical noise analysis. The main advantage of wavelet analysis of EN is the detection of transients which are localized in both the time and frequency domain and shows promise to be discriminatory for the intensity as well as the type of corrosion.

Share on my website

Save to Mendeley

Read in ReadCube

Share on TwitterShare on FacebookShare on LinkedIn

© 2011 The Author(s). Licensee IntechOpen. This chapter is distributed under the terms of the Creative Commons Attribution-NonCommercial-ShareAlike-3.0 License, which permits use, distribution and reproduction for non-commercial purposes, provided the original is properly cited and derivative works building on this content are distributed under the same license.

1839total chapter downloads

Login to your personal dashboard for more detailed statistics on your publications.

Access personal reportingEdited by Hannu Olkkonen

Next chapter#### Applications of Discrete Wavelet Transform in Optical Fibre Sensing

By Allan C. L. Wong and Gang-Ding Peng

Edited by Hannu Olkkonen

First chapter#### Discrete Wavelet Multitone Modulation for ADSL & Equalization Techniques

By Sobia Baig, Fasih-ud-Din Farrukh and M. Junaid Mughal

We are IntechOpen, the world's leading publisher of Open Access books. Built by scientists, for scientists. Our readership spans scientists, professors, researchers, librarians, and students, as well as business professionals. We share our knowledge and peer-reveiwed research papers with libraries, scientific and engineering societies, and also work with corporate R&D departments and government entities.

More About Us